Woodwool Slabs – Manufacture, Properties and Use
Embed Size (px)
Transcript of Woodwool Slabs – Manufacture, Properties and Use
Woodwool Slabs Manufacture, Properties and Useby Erik Johansson
ContentsAcknowledgements 1 Introduction Problem Method Organization of the report 2 General considerations History of woodwool slabs Production Properties Products and uses 3 Recommendations for production Manufacturing process Quality control Plant Equipment Staff Setting up the plant Consumption of raw materials and energy Production costs 4 Choice of wood Technical requirements for the wood Availability of the wood Improving the compatibility of the wood with cement Tests of suitability 5 Properties Thermal properties Strength Acoustic properties Fire performance Moisture properties Durability Emissions of harmful compounds 6 Quality control Size and density Strength Other tests 7 Applications Exterior walls Roofs and ceilings Surface finishes References Appendix 4 4 4 4 4 5 5 5 6 6 7 7 10 10 10 11 12 12 12 14 14 14 14 14 15 15 15 16 16 17 17 17 18 18 18 18 19 19 22 23 24 26 3
Erik Johansson was born in Sweden in 1963. He holds a masters degree in Civil Engineering from Lund University. Since graduation he has done research on building materials, and has participated in development research projects on building technique and building materials in Tunisia, Algeria and Ethiopia. He is engaged as a researcher at Lund Centre for Habitat Studies and at the Division of Building Materials, the Institute of Technology, Lund University. His masters thesis dealt with water leakage in flat roofs in Tunisia, and he wrote a Building Issue on the topic in 1989. He is the house expert on football and spends all his free time out in the Swedish rain cheering on his home team Malm FF.
Volume 6 Number 3
Building Issues 1994
AcknowledgementsI would like to acknowledge some of the help I received during this study. First I would like to thank Mr Bengt Rf (Production Manager) and Mr Lennart Rf of Tepro Byggmaterial, sterbymo, Sweden, for their generous hospitality on the many occasions they invited me, and my colleagues, to their factory and for the time they took to discuss the production and use of woodwool slabs. Invaluable information on the production and use of woodwool slabs was provided by Elten Systems, Barne-veld, the Netherlands, who also commented on the draft report. I am very grateful to Mr John de Wit (Division Manager) and Mr Arnold Plak (Export Manager). My visit to Climatex Indstria de Madeira Minerali-zada, Porto Alegre, Brazil, greatly increased my knowl-edge about woodwool slabs and their use. I would like to thank Mr Carlos Roberto Simm (Operations Direc-tor), Mr Luiz Sergio Bocchese, Mr Werner Dopheide, and Mr Romildo Feij da Rosa for their warm reception, hospitality and willingness to provide information. Last but not least, thanks to Ms Rosane Bauer, Architect, who participated in the Architecture & Development course at LCHS in 1993. She acted as guide and translator during my visit to Porto Alegre. Erik Johansson
1 IntroductionProblemThermal insulation is important to improve indoor climate and save energy in a building. The use of thermal insulation materials are, however, often limited in developing countries. There are several reasons, for example: The advantages of thermal insulation materials are not known. Local thermal insulation materials are not available. Imported thermal insulation materials are expensive and require foreign currency. Use of thermal insulation materials requires modification in current building methods. This reports deals with woodwool slabs, a well tested thermal insulation material that can be made locally in most countries. Because of their versatility, woodwool slabs are easy to integrate with most construction techniques. Many of the materials traditionally used in contemporary buildings bricks, concrete, stone, soil block, etc. have poor thermal insulation capacity. To reach the same thermal insulation as 100 mm of woodwool slab requires about 4 m natural stone, 1.8 m concrete, 700 mm soil block or concrete hollow block and 500 mm hollow brick.
MethodThis report is primarily based on the experience gained from a research cooperation between Lund University, Division of Building Materials and LCHS, and the National Centre for Building Research and Studies (CNERIB) in Algeria during the period 19911993. This project, which included test production of wood-wool slabs with Algerian woods and full scale tests of the slabs in building components, laid the foundation for introducing woodwool slabs on the Algerian market. Visits were made to modern, completely automated factories in Sweden and the Netherlands. A semi-automated, labour intensive factory was studied in Brazil. Detailed studies were also made on the use of woodwool slabs in these countries. The report is also based on a study of the literature, including a large part of all the material on woodwool slabs written over the years.
Organization of the reportThe report is divided into two parts. The first part includes Chapter 1, the background to the study, Chapter 2, a short description of the production, properties and use of woodwool slabs, and Chapter 3, a description of how woodwool slabs can be produced industrially in developing countries. The second part includes Chapter 4, choosing an appropriate wood, Chapter 5, the properties of woodwool slabs, Chapter 6, quality control, and Chapter 7 examples of use. 4
Building Issues 1994
Volume 6 Number 3
2 General considerationsHistory of woodwool slabsSlabs of woodwool (excelsior), gypsum and water were patented in Germany already in 1880. During the 1910s production of woodwool slabs with magnesite as the binding agent (patented 1908) started in Austria. Magnesite1 gave better durability than gypsum. Portland cement was introduced at the end of the 1920s, and is the most common binder today, which is why they are commonly called woodwool cement slabs and, in North America, cement excelsior boards (CEB). For a long time woodwool slabs were made in Germany with either gypsum, magnesite or cement as binder. Gypsum slabs are no longer made. The technique to produce woodwool slabs mainly cement-bonded, but even magnesite-bonded spread quickly from Austria and Germany to other European countries and North America. A great increase in production occurred during the years before and after the second world war, and woodwool slabs were spread even farther geographically. At first cement-bonded woodwool slabs were produced by hand in small plants. The equipment was limited to wood shredding machines, to make the woodwool, and a mixer. Manufacture became more and more mechanized over the years, with significantly high production capacity. Modern factories are normally fully mechanized, and about 15 persons can produce up to 150 m3 slabs a day. The most commonly used wood for woodwool slabs comes from conifers, mainly pines and firs. During the 1960s a great number of other species were tested, including tropical woods, to see if they could be used for woodwool slabs. A number of species were suitable, which led to production of woodwool slabs on other continents. There is currently production in Africa (Ghana, Malawi, Namibia, Zambia), Asia (Burma, India, Indonesia, Japan, Malaysia, the Philippines, Taiwan, Thailand) and Latin America (Brazil, Mexico, Panama, Peru, Venezuela). Production in these countries varies in the degree of mechanization everything from manual to completely automated.
Fig. 1 Making woodwool in a vertical wood shredding machine (Tepro, Sweden). Shredders sold today are horizontal. See Figs 9 and 10.
duces the amount of sugar and other compounds in the wood that inhibit setting of the slabs, and lowers the moisture content (shredding is more difficult with green wood). To make woodwool, a half metre long log is placed in a shredding machine (Fig. 1) fitted with scoring knives perpendicular to the planing knives. The cross section of the woodwool is determined by adjusting the speed with which the log is fed toward the planing knife, and the distance between the scoring knives. The thickness of the woodwool can vary between 0.2 0.5 mm, and the width between 1.5 5 mm depending on how the slab will be used. The amount of woodwool in a slab varies between about 75 200 kg depending on the density of the slab. Binder The most commonly used binder in woodwool slabs is Portland cement, but magnesite can also be used. The Portland cement is normally of ordinary type (OPC), although rapid-hardening cement can be used to make the setting faster. Sometimes white cement is used for aesthetic reasons. For magnesite-bonded slabs the binder can be said to be magnesium oxide (MgO), one of the components of magnesia cement. The amount of binder depends on the density of the woodwool slab, and varies between about 150 and 400 kg/m3. Binder additives Normally some kind of binder additive is necessary. The setting of the Portland cement and water mixture can be inhibited to greater or lesser extent by sugars and other chemicals in the woodwool. An accelerator is therefore often added so that the slabs set within 24 hours. The most common accelerator is calcium chloride (CaCl2). The amount of accelerator depends on the kind of wood, but is usually about 2% by weight of the water. For magnesite-bonded slabs the binder additive is either magnesium chloride (MgCl2) or magnesium sulphate (MgSO4).
ProductionThe components needed for woodwool slabs are woodwool, binder (Portland cement or magnesite) and water. Normally a small amount of binder additive is added to speed up setting. Making woodwool Woodwool can be made from a number of woods. To make production easier, the wood should allow easy shredding (have a low density) and not contain compounds that seriously inhibit the setting of the slab. Usually the tree trunks are air-dried (seasoned) before cutting into logs and shredding to